Evaluation of a New and Advance Curing Light IJOCR
Evaluation of a New and Advance Curing Light on the
Shear Bond Strength of Orthodontic Brackets
1Amit Bithu, 2Arvind Singh Bithu, 3Mahesh Aghera
ORIgInal ReseaRCh 10.5005/jp-journals-10051-0121
Keywords: Curing lights, Light-emitting diode/halogen, Orth-odontic brackets, Shear bond.
How to cite this article: Bithu A, Bithu AS, Aghera M. Evaluation of a New and Advance Curing Light on the Shear Bond Strength of Orthodontic Brackets. Int J Oral Care Res 2017;5(4):305-309. Source of support: Nil
Conflict of interest: None
Bonding of brackets to enamel has been a critical issue in orthodontic research, since the significance of achieving a stable bond between the tooth and its bracket is very important. Biomechanical principles required a relatively inelastic interface that would transfer a load applied to the bracket, due to engagement of an activated arch wire to the tooth without exceeding its bond strength.1,2
Clinicians soon became aware of problems related to low bond strength and the resulting necessity of repeating the bonding procedure as treatment progressed. Early bonding systems consisted of brackets welded into bands bonded to enamel with zinc phosphate cement. Apart from esthetic considerations, this approach presented other serious disadvantages:
• The requirement of extensive chair time.
• The necessity of frequent screening for development of caries or decalcification of underlying tooth structure. • The pronounced effect on periodontal health due
to chemical and mechanical irritation of the gingiva caused by cements and the accumulated plaque. • The requirement of additional arch space to
accom-modate band placement, thus affecting consideration of extraction in borderline cases.
Therefore, the need of finding an alternative proce-dure was felt after understanding the aforementioned drawbacks of banding which would provide retention of the brackets to tooth enamel. One of the most dramatic changes in the orthodontic specialty in the 1970s was the use of composite resin as a bonding material. The use of self-cured composite resin for direct bonding of orthodontic brackets to the tooth surface was then well documented. For years, the use of self-cured orthodontic resin was the only choice for direct bonding. The polym-erization of self-cured resin with the two-paste system or the one-paste system starts immediately on mixing; thus,
1Department of Orthodontics, Jodhpur Dental College and General Hospital, Jodhpur, Rajasthan, India
2Department of Prosthodontics, Jodhpur Dental College and General Hospital, Jodhpur, Rajasthan, India
3Department of Orthodontics, Darshan Dental College & Hospital, Udaipur, Rajasthan, India
Corresponding Author: Amit Bithu, Senior Lecturer, Department of Orthodontics, Jodhpur Dental College and General Hospital Jodhpur, Rajasthan, India, e-mail: email@example.com ABSTRACT
Introduction: With the introduction of photosensitive (light-cured) restorative materials in dentistry, various methods were suggested to enhance their polymerization and curing time including layering and the use of more powerful light curing devices. The purpose of this study was to comparatively evalu-ate shear bond strength of stainless steel bracket using conven-tional halogen light and light-emitting diode (LED) curing units. Materials and methods: This in vitro study was carried out
in the Department of Orthodontics, Pacific Dental College,
Debari, Udaipur, India. Sample included 120 freshly extracted human premolars collected and etched by 37% phosphoric acid, washed and dried, and sealent applied. Then preadjusted edgewise upper premolar stainless steel brackets were applied on the teeth. The teeth were divided into groups of six, each group having 20 teeth. Group I was cured by halogen light curing unit by 10 seconds, group II is cured by LED curing unit by 10 seconds, group III is cured by halogen light curing unit by 20 seconds, group IV is cured by LED curing unit by 20 seconds, group V is cured by halogen light curing unit by 40 seconds, group VI is cured by LED curing unit by 40 seconds.
Result: One-way analysis of variance (ANOVA) showed that p
score was significant at <0.001, which indicated that all the six groups differ significantly. This was further investigated using multiple range test by Tukey’s honest significant difference
(HSD) procedure in Table 4. And it was observed that mean
shear bond strength in group I was significantly lower than the mean shear bond strength in groups II to VI (p < 0.05). Also, the mean shear bond strength in group II was significantly
lower than the mean shear bond strength in groups III to VI
(p < 0.05).
Conclusion: It is concluded that 10 seconds of curing time is not adequate for both halogen and LED light. Twenty seconds of curing time is adequate for both LED and halogen light, since
increasing the curing time to 40 seconds showed no significant
tooth surface. The air bubbles that arise during mixing or the uneven consistencies in resins that are mixed by hand result in the weakening of the bond strength in the two-paste system.3-6
Then ultraviolet light-cured materials were intro-duced and quickly replaced those products that were self-cured. These ultraviolet light-cured materials have the disadvantages of radiation hazards and limited depth of cure. These problems have been largely overcome by the introduction of a blue, visible light-cured composite resin. Compared with ultraviolet light, visible light has deeper curing capabilities, is more effective through enamel, and does not diminish with time or with the intensity of the light source.7,8
With time, desire to cure on demand is driving an increasing number of orthodontic practices to utilize light cure adhesives instead of the more traditional two-paste adhesives requiring in-office mixing. Now light-cured adhesives are routinely used for bonding in orthodontics. The greatest advantage of a light-cured adhesive system is that it gives the clinician ample time to accurately posi-tion the bracket on the enamel surface before using the light to polymerize the adhesive.9
Light-cured orthodontic adhesives have been used almost exclusively with light emitted from a halogen source. However, tungsten–quartz halogen curing units have several shortcomings. They have a harmful effect on teeth pulp, especially when used in orthodontic practice where most of patients are from younger age group with large pulp chambers. Only 1% of the total energy input is converted into light and the remaining is generated as heat. The short life of halogen bulbs, noisy cooling fan, and the time it takes to expose each bonded bracket to the light (10–40 seconds) are other disadvantages.
However, up to 40 seconds of curing time per bracket has been recommended to allow for adequate polymeriza-tion with a convenpolymeriza-tional halogen light source, resulting in a considerable amount of chair time if one or both arches are bonded to overcome these problems. Light curing units with gallium nitride blue LEDs have been proposed for curing resin-based dental adhesives. The spectral output of LEDs falls within the absorption spec-trum of camphorquinone, so the LEDs require no filters to produce blue light. Mills et al were among the first to suggest the use of solid-state LEDs for the polymeriza-tion of light-sensitive dental materials. The use of LED technology has two major advantages, namely, avoiding the use of the heat-generating halogen bulbs and the fact that they have 10,000 hours lifetime with little degrada-tion of output.
produced by the halogen curing unit sources was larger than that obtained with the LEDs. Furthermore, advance-ments in the power output of LEDs have allowed them to achieve a higher irradiance than halogen curing units.10
These high-intensity LEDs may decrease total light curing time.
The aim of this study was
• To evaluate shear bond strength of stainless steel bracket cured with two different lights, i.e., halogen and commercially available LED curing units. • To establish the optimum curing time while using
LED curing light.
MATERIALS AND METHODS Teeth
One hundred and twenty freshly extracted human upper premolars were collected and stored in a solution of 1% (wt/vol) thymol. The criteria for tooth selection included intact buccal enamel, not subjected to any pretreatment chemical agents like hydrogen peroxide, with no cracks, due to the pressure of the extraction forceps, and no caries. The teeth were cleansed and polished with pumice and rubber prophylactic cups for 10 seconds.
The buccal surface of enamel of each tooth was condi-tioned for 20 seconds with 37% phosphoric acid gel. Each tooth was then rinsed with a water spray for 20 seconds and dried with oil-free air for 10 seconds. The buccal enamel surfaces of the etched teeth appear chalky white.
Preadjusted edgewise upper premolar stainless steel brackets (0.22 Roth prescription, 3M Unitek Gemini series) were used. The average surface area of the bracket base was 11.8 mm2.
One hundred and twenty teeth were randomly divided into six equal groups that were bonded according to time and different type of curing lights (Table 1). The curing lights were halogen light curing unit (Elipar 2500, 3M-ESPE, Seefeld, Germany) and LED curing unit (Woodpecker).
Evaluation of a New and Advance Curing Light IJOCR
Shear Bond Strength
Debonding was carried out with Universal Testing Machine (Instron), load cell = 1 KN. The machine has two vertically placed jaws. The acrylic block with the tooth embedded was placed in the lower jigs.
The embedded teeth and brackets were aligned in the testing apparatus to ensure consistency for the point of force application and direction of the debonding force for all specimens. The shear-peel force was applied with a custom-made chisel-shaped rod from the occlusal side parallel to the bracket surface between the bracket base and the tie wings.
An occlusogingival load was applied to the bracket producing a shear force at the bracket–tooth interface. A computer electronically connected with the Instron Universal Testing Machine recorded the results of each test. Shear bond strengths were measured at a crosshead speed of 1 mm/min.
The Instron Universal Testing Machine unit was attached to an electronic console that displayed the debonding forces acting between the jaws. Thus, the exact force at which the bracket debonded was noted from the console. This force was expressed in Newtons.
The results obtained from the shear bond strength testing of metal brackets cured by two different light curing units were tabulated. Their mean and standard deviation (SD) were calculated and then subjected to following statisti-cal evaluation to determine the statististatisti-cal significance of the present study. The following statistical evaluation was done:
• one-way ANOVA test
• multiple range test by Tukey’s HSD procedure • Kaplan–Meier survival analysis
The mean and SD value of shear bond strength of stain-less steel bracket cured with halogen for 10 seconds (group I) shown in Table 2 is 1.172 ± 0.869 MPa. The mean and SD value of shear bond strength of stainless steel bracket cured with LED for 10 seconds (group II) is 4.719 ± 1.766 MPa. The mean and SD value of shear bond strength of stainless steel bracket cured with halogen for 20 seconds (group III) is 7.824 ± 2.617 MPa. The mean and SD value of shear bond strength of stainless steel bracket cured with LED for 20 seconds (group IV) is 7.534 ± 2.682 MPa. The mean and SD value of shear bond strength of stainless steel bracket cured with halogen for 40 seconds (group V) is 8.261 ± 2.390 MPa. The mean and SD value of shear bond strength of stainless steel bracket cured with LED for 40 seconds (group VI) is 8.489 ± 2.373 MPa.
One-way ANOVA analysis in Table 3 shows that p-value was found significant at <0.001, which indicated that all the six groups differ significantly.
This was further investigated using multiple range test by Tukey’s HSD procedure in Table 4. And it was observed that mean shear bond strength in group I was significantly lower than the mean shear bond strength in groups II to VI (p < 0.05). Also, the mean shear bond strength in group II was significantly lower than the mean shear bond strength in groups III to VI (p < 0.05).
Hence, this study shows that shear bond strength in group I was significantly lower than the shear bond strength in groups II to VI. Also, the shear bond strength in group II was significantly lower than the mean shear bond strength in groups III to VI. However, there was no significant difference between any other contrasts. • Therefore, it is concluded that 10 seconds of curing
time is not adequate for both halogen and LED light. • Twenty seconds of curing time is adequate for both
LED and halogen light, since increasing the curing time to 40 seconds showed no significant difference.
Table 1: Number of teeth, color, time and light used to cure among different study groups
teeth Color Time (seconds) Light used to cure
Group I, 20 White 10 Halogen
Group II, 20 Yellow 10 LED
Group III, 20 Green 20 Halogen
Group IV, 20 Red 20 LED
Group V, 20 Blue 40 Halogen
Group VI, 20 Black 40 LED
Table 2: Mean, SD, and test of significance of mean values
between different study groups
Groups Mean ± SD (MPa)
groups at 5% level Group I 1.712 ± 0.869 Halogen VI, V, IV, III,
II vs I, VI, V, IV, III vs II Group II 4.719 ± 1.766 LED
Group III 7.824 ± 2.617 Halogen Group IV 7.534 ± 2.682 LED Group V 8.261 ± 2.390 Halogen
Group VI 8.489 ± 2.373 LED <0.0001 (significant)
*One-way ANOVA was used to calculate the p-value; #Multiple range
test by Tukey’s HSD procedure was employed to identify significant
groups at 5% level
Table 3: Analysis of variance
Bond strength Sum of squares df Mean square F Significance
Between groups 825.333 5 165.067 33.851 0.000 Within groups 555.897 114 4.876
The results of this study are promising for the orth-odontic application of LED curing units, but further compatibility and physical characteristic studies of various orthodontic adhesives and clinical trials should be performed before validation.
DISSCUSSION AND CONCLUSION
To achieve more effective photoactive and cure dental adhesives, various types of lights have been used includ-ing the newly introduced Turbo tips.11-13 These turbo
tips were not too effective for orthodontic purposes.13
Ideally, the early, i.e., more effective, cure should result in less stress at the enamel–adhesive interface during the initial ligation of arch wires. Therefore, any enhance-ment to the initial curing by a more effective method of photoactivation is intended to help bond the adhesive to the tooth faster.12
Mills et al14 studied the difference in depth of cure and
compressive strength of dental composites cured with either a LED-based light curing unit or a conventional halogen-based light curing unit.
The irradiance and emitted light spectra were also measured for both light curing units. No statistically significant difference in compressive strength was found between samples cured with halogen or the LED light curing units. Depth of cure for the halogen light curing unit was about 20% higher than that obtained for LED light curing unit. The difference in irradiance of the two types of light curing units is large but only a small difference in depth of cure was found. A good correlation was found between the absorption spectrum of camphoroquinone and the spectrum of the LED light curing unit. The advantage of the LED light curing device
is that the clinician is able to light cure two orthodontic brackets with the same light exposure without signifi-cantly influencing the shear bond strength. This approach reduces the total curing time by half when bonding orth-odontic brackets with photosensitive. Our study showed that LED is a viable alternative to halogen light curing unit in spite of its reduced irradiance. Although the LED does not cure faster than the halogen light curing units, it is a much less expensive alternative to xenon light and argon laser. While the cost is comparable to conventional halogen light, they have additional advantages of low maintenance cost, half the heat production of halogen lights, and are lighter and portable.15-17
Therefore, it is concluded that 10 seconds of curing time is not adequate for both halogen and LED lights. Twenty seconds of curing time is adequate for both LED and halogen light, since increasing the curing time to 40 seconds showed no significant difference.
The LED can be considered as useful tool for ortho-dontist to save bonding time. The LED light units are cordless, smaller, and lighter with estimated lifetimes of over 10,000 hours, and they do not require a noisy cooling fan. Therefore, it seems that they are a better choice as compared with halogen sources. Further investigation under clinical conditions is suggested to compare the results to previous in vitro studies.
1. Ruyter IE, Gyorosi PP. An infrared spectroscopic study of sealants. Scand J Dent Res 1976 Nov;84(6):396-400.
2. Fan PL, Stanford CM, Stanford WB, Leung R, Standford JW. Effects of backing reflectance and mold size on polymeriza-tion of photo-activated composite resin. J Dent Res 1984 Oct;63(10):1245-1247.
1.00 2.00 –3.54700* 0.69830 0.000 –5.5712 –1.5228
3.00 –6.65200* 0.69830 0.000 –8.6762 –4.6278
4.00 –6.36150* 0.69830 0.000 –8.3857 –4.3373
5.00 –7.08850* 0.69830 0.000 –9.1127 –5.0643
6.00 –7.31650* 0.69830 0.000 –9.3407 –5.2923
2.00 3.00 –3.10500* 0.69830 0.000 –5.1292 –1.0808
4.00 –2.81450* 0.69830 0.001 –4.8387 –0.7903
5.00 –3.54150* 0.69830 0.000 –5.5657 –1.5173
6.00 –3.76950* 0.69830 0.000 –5.7937 –1.7453
3.00 4.00 0.29050 0.69830 0.998 –1.7337 2.3147
5.00 –0.43650 0.69830 0.989 –2.4607 1.5877
6.00 –0.66450 0.69830 0.932 –2.6887 1.3597
4.00 5.00 –0.72700 0.69830 0.903 –2.7512 1.2972
6.00 –0.95500 0.69830 0.746 –2.9792 1.0692
5.00 6.00 –0.22800 0.69830 0.999 –2.2522 1.7962
Evaluation of a New and Advance Curing Light IJOCR
3. Ruggeberg FA, Caughman WF, Curtis JW, Davis HC. A pre-dictive model for the polymerization of photo-activated resin composites. Int J Prosthodont 1994 Mar-Apr;7(2):159-166. 4. Johnston WM, Leung RL, Fan PL. A mathematical model
for post-irradiation hardening of photo-activated composite resins. Dent Mater 1985 Oct;1(5):191-194.
5. Leung RL, Fan PL, Johnston WM. Post-irradiation of visible light activated composite resin. J Dent Res 1983 Mar;62(3):263-265. 6. Rueggeberg FA, Caughman WF, Curtis JW. Effect of intensity
and exposure duration on cure of resin composite. Oper Dent 1994 Jan-Feb;19(1):26-32.
7. Blankeneau RJ, Kelsey WP, Powell GL, Shearer GO, Barkmeir WW, Cavel WT. Degree of composite resin polymerization with visible light and argon laser. Am J Dent 1991 Feb;4(1):40-42. 8. Cacciafesta V, Sfondrini MF, Sfondrini G. A xenon arc
light-curing unit for bonding and bleaching. J Clin Orthod 2000;34:94-96.
9. Hannig M, Bott B. In vitro pulp chamber temperature rise during composite resin polymerization with various light curing sources. Dent Mater 1999 Jul;15(4):275-281.
10. Zach L, Cohen J. Pulp response to externally applied heat. Oral Surg Oral Med Oral Pathol 1965 Apr;19:515-530. 11. Clinical Research Associates Newsletter. United states 2000;
12. Curtis JW, Rueggeberg FA, Lee AJ. Curing efficiency of the Turbo tip. Gen Dent 1995 Sep-Oct;43(5):428-433.
13. Bishara SE, VonWald L, Laffoon JE. Standard vs. Turbo light guides and their effects on the shear bond strength of an ortho-dontic adhesive. World J Orthod 2001 Summer;2(2):154-158. 14. Mills RW, Jandt KD, Ashworth SH. Dental composite depth of
cure with halogen and blue light emitting diode technology. Br Dent J 1999 Apr;186(8):388-391.
15. Nakamura S, Mukai T, Senoh M. Candela-class high brightness in GaN/AlGaN double heterostructure blue-light-emitting diodes. Appl Phys Lett 1994 Jun;64:1687-1689.
16. Haitz RH, Craford MG, Wiessman RH. Handbook of optics. Vol. 2. New York, NY: McGraw Hill; 1995. p. 12.1-12.9. 17. Dunn WJ, Taloumis LJ. Polymerization of orthodontic resin